Nanocasting Synthesis of Ultrafine WO3 Nanoparticles for Gas Sensing Applications
- First Online:
- Cite this article as:
- Kamali Heidari, E., Marzbanrad, E., Zamani, C. et al. Nanoscale Res Lett (2010) 5: 370. doi:10.1007/s11671-009-9490-8
- 4.7k Downloads
Ultrafine WO3 nanoparticles were synthesized by nanocasting route, using mesoporous SiO2 as a template. BET measurements showed a specific surface area of 700 m 2/gr for synthesized SiO2, while after impregnation and template removal, this area was reduced to 43 m 2/gr for WO3 nanoparticles. HRTEM results showed single crystalline nanoparticles with average particle size of about 5 nm possessing a monoclinic structure, which is the favorite crystal structure for gas sensing applications. Gas sensor was fabricated by deposition of WO3 nanoparticles between electrodes via low frequency AC electrophoretic deposition. Gas sensing measurements showed that this material has a high sensitivity to very low concentrations of NO2 at 250°C and 300°C.
KeywordsWO3 Nanocasting Low frequency AC electrophoretic deposition NO2 gas sensor
Semiconductor gas sensors offer good advantages with respect to other gas sensor devices due to their simple implementation, low cost and good reliability for real-time control systems [1, 2, 3]. Among them, ZnO, WO3 and SnO2 have widely been studied . Tungsten oxide (WO3) is a wide band gap, n-type semiconductor that has interesting physical and chemical properties [5, 6, 7, 8, 9]. WO3 is a good photochromic, electrochromic, thermochromic and catalytic material [9, 10, 11, 12].
Gas sensing is a surface effect. As gas adsorption occurs at surface level, an increase in the active surface area of the semiconductor oxide would enhance the properties of materials used as gas sensors [4, 13, 14, 15]. Nanostructured mesoporous materials have been widely studied in the development of gas sensing and catalytic systems, due to their large, controllable pore size and high surface area [1, 13, 16, 17, 18]. Nanocasting is a novel methodology for preparing nanoparticles by using mesoporous materials as a template to accommodate different oxides. In this synthesis pathway, the surface and voids of a preformed mesoporous solid are coated with desired precursors. The subsequent mineralization of these precursors and removal of the former solid templates may lead to mesostructures with other compositions and crystalline frameworks [1, 13, 19].
While using in chemical sensors, the sensing material should be aligned and connected between the electrode structures, so that the change of their properties is converted into electrical signal, when exposed to the measurand. Several approaches have been reported in the literature for placement of the nanomaterials between the electrodes, but most of them do not offer selective settlement of particles or need expensive apparatus and high vacuum . Using electric field is one of the most versatile techniques known till date for selective and inexpensive assembly of nanoparticles .
In this research, we applied a nanocasting route for synthesis of ultrafine WO3 nanoparticles. In the first step, mesoporous silica (SBA-15 structure) was prepared using a soft template, and in the second step, this material was used as a hard template in nanocasting of WO3 nanoparticles. Also, alternating electric field was used to manipulate the sensing material between electrodes, in order to fabricate gas sensor.
Mesoporous SiO2 was synthesized, using bottom-up method. Polyethylene oxide–polypropylene oxide block copolymer was used as soft template and tetraethyl orthosilicate (TEOS) as silicate source. In the first step, 6 gr of the copolymer, 180 cc distilled water and 30 gr HCl (35% wt) were mixed together, and the solution was stirred for 6 h at 35°C. In the second step, TEOS was added to this acidic solution and stirred for 24 h at the same temperature and then heated at 100°C for another 24 h as a hydrothermal treatment. Small volume of NH3 was added in order to increase the PH up to 7. Then, the product was dried at room temperature in air atmosphere and calcined at 550°C for 4 h. The solid product of this process is mesoporous SiO2, which will be used as nanotemplate in production of WO3 nanoparticles.
The synthesis of WO3 nanoparticles was carried out as follows: equal amounts of phosphotungstic acid hydrate and mesoporous SiO2 were dissolved in ethanol, stirred vigorously for 1 h, dried at room temperature at air atmosphere and heated at 570°C for 5 h. The SiO2 hard template was removed by HF (2% wt), and the product was collected by centrifugation. The product was washed both with water and ethanol for three times and dried at room temperature.
For sensor fabrication, WO3 nanopowders were deposited on an alumina substrate between electrodes, via low frequency AC electrophoretic deposition [21, 22, 23]. For this purpose, a suspension of 1 gr/l WO3 nanoparticles in acetone was prepared and ultrasonicated for 15 min to become stable and homogenous. Deposition was done by applying a voltage of 25 v and a frequency of 1 KHz. The sensor was calcined for 1 h at 58°C in an electric furnace and air atmosphere.
Synthesized powders were characterized by X-ray diffraction (XRD, Siemens D500, cu Kα radiation) and transmission electron microscopy (HRTEM, JEOL2000 and TEM, Phillips). Nitrogen adsorption–desorption measurements were done using Gemini2375 instrument to determine the Brunauer–Emmett–Teller (BET) surface area. Response of the sensors toward various concentrations of NO2 was measured using a normal set-up. The gas response was calculated as Ra/Rg, where Ra and Rg represent samples’ resistances without and with the presence of gas, respectively.
Results and Discussion
BET measurements showed a surface area of about 700 m 2/gr for mesoporous SiO2 template that was reduced to 43 m 2/gr for WO3 nanoparticles.
Sensing test results prove that the synthesized nanoparticles are sensitive to low concentrations of NO2, which may be a consequence of ultrafine particle size that leads to higher active surface. Application of electric field for deposition of particles also improves the sensing properties of the fabricated gas sensor, thanks to precise placement of particles side by side and establishment of a good connection between the electrodes facilitating the charge transfer between electrodes.
Ultrafine WO3 nanoparticles rather uniform in diameter (∼5 nm) were synthesized efficiently by nanocasting route. AC electrophoresis was applied to deposit WO3 nanoparticles between electrodes in order to fabricate the gas sensor. The sensing measurements showed that the synthesized particles are sensitive even to very low concentrations of NO2(100 ppb), which is a result of very small particle size combined with application of proper deposition method.